Download presentation

Presentation is loading. Please wait.

Published byLisandro Bank Modified over 3 years ago

1
S-1PAT321, Section, June 2002 SECTION COMPOSITE MATERIALS

2
S-2PAT321, Section, June 2002 COMPOSITE MATERIALS n Classical Lamination Theory n Composite Material Definition n QUAD4 and TRIA3 elements n Ply Data Recovery n Composite Failure Theorems Post Processing Not Supported in MSC.PATRAN

3
S-3PAT321, Section, June 2002 Ply Definition n Typically a ply is a flat group of fibers imbedded in a matrix. n The matrix is usually an isotropic material that holds the fibers together. n In a ply called a tape, the fibers are unidirectional. n In a ply called a cloth, the fibers are woven at 0 and 90 degree directions.

4
S-4PAT321, Section, June 2002 Tape Plies n Fiber: u Unidirectional in tape u direction is the 1 axis of the ply coordinate system n Matrix: u glue that holds fibers together u matrix direction is the 2 axis u 90 degrees to the 1 axis n Material properties are: u 2D orthotropic material in Patran u MAT8 in Nastran

5
S-5PAT321, Section, June 2002 MAT8 bulk data entry n Defines the ply orthotropic properties. u Elastic properties are E1, E2, NU12, G12, G1Z, G2Z. u Allowables are Xt, Xc, Yt, Yc, S. u Use STRN if allowables are in units of strain. u F12 is for the Tsai-Wu failure theorem. u Thermal coefficients of expansion are A1 and A2, u initial temperature is TREF, u density is RHO, u damping is GE. n The example below is typical for a graphite/epoxy tape. 12345678910 MAT8MIDE1E2NU12G12G1ZG2ZRHO MAT8 120.+62.+60.351.5+61.6+61.4+61.3-4 A1A2TREFXtXcYtYcS -2.3-74.5-60.01.1+51.05+51.2+41.5+42.+4 mat8, 1, 20.+6, 2.+6, 0.35, 1.5+6, 1.6+6, 1.4+6, 1.3-4,+ +, -2.3-7, 4.5-6,, 1.1+5, 1.05+5, 1.2+4, 1.5+4, 2.+4.bdf file extract GEF12STRN

6
S-6PAT321, Section, June 2002 Patran 2D Orthotropic Materials: Create/ 2d Orthotropic/ Manual Input Material Name Input Properties Linear Elastic Apply Input Properties Failure Apply

7
S-7PAT321, Section, June 2002 Composite Material n Stack of plies n Each ply has a different direction, material, and thickness n Composite properties are calculated in the material coordinate system (Xm, Ym, Zm) n Zm is the same as the element Z axis (Ze) n Xm is either an angle relative to element G1G2 vector or is the projection of the X axis of a defined coordinate system n Positive angles are defined by right hand rule around Zm

8
S-8PAT321, Section, June 2002 PCOMP bulk data entry n Defines the composite layup. n The example composite below is an 8 ply layup, symmetric about its centerline, with an equal number of plies is each of the 0, +-45, 90 degree directions. 12345678910 PCOMPPIDZ0NSMSBFTTREFGELAM PCOMP 1 5000.0HILL0.0 MID1T1THETA1SOUT1MID2T2THETA2SOUT2 10.00540.0YES10.005445.0YES pcomp,1,,,5000.0,hill,,,,+ +,1,.0054, 0.0,yes,1,.0054, 45.,yes,+ +,1,.0054,-45.,yes,1,.0054, 90.,yes,+ +,1,.0054, 90.,yes,1,.0054,-45.,yes,+ +,1,.0054, 45.,yes,1,.0054, 0.0,yes.bdf file extract MID3T3THETA3SOUT3ect. 10.005490.0

9
S-9PAT321, Section, June 2002 Patran Composite Materials: Create/ Composite/ Laminate Click on tape property name for each of the plies Thickness for all layers:.0054 Orientations: 0 45 –45 90 90 –45 45 0 Load Text Into Spreadsheet Apply

10
S-10PAT321, Section, June 2002 CQUAD4 bulk data entry n Defines the composite plate. n Material coordinate system can be defined one of two ways: u MCID – (integer) - ID of a user defined coordinate system whos X-axis is projected onto the element to define the elements material coordinate systems X- axis. This along with the Z-axis of the element coordinate system defines the material coordinate system. u THETA – (real) - an angle between the G1G2 vector of the element and the X-axis of the material coordinate system. The positive sense of this angle is the right hand rule direction around the elements Z-axis. 12345678910 CQUAD4EIDPIDG1G2G3G4THETA or MCID ZOFFS CQUAD4 11123499 cquad4,1,1,1,2,3,4,99 cquad4,1,1,1,2,3,4,25.0

11
S-11PAT321, Section, June 2002 Patran Composite Properties Properties: Create/ 2D/ Shell Option: Laminate Input Properties Click on composite material name Click on coord. sys. for projection to material coord. sys. OK Select elements Apply

12
S-12PAT321, Section, June 2002 Patran Material Coord. Z-axis Elements: Verify/ Element/ Normals Draw Normal Vectors Apply

13
S-13PAT321, Section, June 2002 Patran Material Coord. X-axis Properties: Show/ Shell Orientation Angle Apply

14
S-14PAT321, Section, June 2002 Patran Ply Output Request Analysis: Analyze/ Entire Model/ Full Run Subcases/ Create Output Requests/ Advanced/ Element Stress Ply Stresses OK Apply

15
S-15PAT321, Section, June 2002 Patran Ply Stress Results Attach xdb: Results: Create/ Quick Plot Result/ Stress Tensor Position/ Layer 1 Quantity/ X Component Apply

16
S-16PAT321, Section, June 2002 Composite Failure Indices n Hill: 1, 2, 12 are ply stresses from the Nastran analysis X, Y, S are ply stress allowables from the PCOMP bulk data entry F 12 is experimentally determined n Hoffman: n Tsai-Wu:

17
S-17PAT321, Section, June 2002 Composite Failure Indices n Max Strain: u Three failure indices u One for each direction u Uses strain allowables 1, 2, 12 are ply strains from the Nastran analysis X, Y, S are ply strain allowables from the PCOMP bulk data entry (set STRN term on PCOMP to 1.0) 1, 2, 12 are ply stresses from the Nastran analysis X, Y, S are ply stress allowables from the PCOMP bulk data entry n Max Stress: u Same as Max Strain but allowables are in stress units

18
S-18PAT321, Section, June 2002 F A I L U R E I N D I C E S F O R L A Y E R E D C O M P O S I T E E L E M E N T S ( Q U A D 4 ) ELEMENT FAILURE PLY FP=FAILURE INDEX FOR PLY FB=FAILURE INDEX FOR BONDING FAILURE INDEX FOR ELEMENT FLAG ID THEORY ID (DIRECT STRESSES/STRAINS) (INTER-LAMINAR STRESSES) MAX OF FP,FB FOR ALL PLIES 1 HILL 1 6.6183 0.1776 2 4.1766 0.1822 3 14.5333 0.0315 4 20.0144 20.0144 *** 2 HILL 1 1.8251 0.1288 2 0.9096 0.1322 3 4.0140 0.0228 4 9.5973 9.5973 *** 3 HILL 1 6.0914 0.1912 2 8.4410 0.1961 3 7.4905 0.0339 4 10.2642 10.2642 *** 4 HILL 1 0.0641 0.1153 2 0.8806 0.1183 3 8.7623 0.0204 4 19.9326 19.9326 *** Nastran Failure Index Output n Printed in the f06 file if allowbles on PCOMP bulk data entry are present. n Failure index display not supported in Patran..f06 file extract

Similar presentations

OK

MULTIPLICATION EQUATIONS 1. SOLVE FOR X 3. WHAT EVER YOU DO TO ONE SIDE YOU HAVE TO DO TO THE OTHER 2. DIVIDE BY THE NUMBER IN FRONT OF THE VARIABLE.

MULTIPLICATION EQUATIONS 1. SOLVE FOR X 3. WHAT EVER YOU DO TO ONE SIDE YOU HAVE TO DO TO THE OTHER 2. DIVIDE BY THE NUMBER IN FRONT OF THE VARIABLE.

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on google driverless cars Ppt on automobile related topics such Ppt on ozone depletion and global warming Ppt on high level languages pascal Ppt on johari window model+example Ppt on places in our neighbourhood download Ppt on product specification for food Ppt on asymptotic notation of algorithms to solve Ppt on project spark Ppt on bluetooth vs wifi